J. Phys. Chem. C 2010, 114, 10403–10409
Femtosecond Laser Synthesis of AuAg Nanoalloys: Photoinduced Oxidation and Ions Release Se´bastien Besner and Michel Meunier* Laser Processing Laboratory, Department of Engineering Physics, E´cole Polytechnique de Montre´al, CP6079, Succ. Centre-Ville, Montre´al, QC, Canada H3C 3A7 ReceiVed: March 18, 2010; ReVised Manuscript ReceiVed: May 7, 2010
A femtosecond laser irradiation approach has been developed for the production of homogeneous AuAg nanoalloys of various compositions. The mean size was controlled by the dextran-nanoparticle affinity and resulted in the production of 5-7 nm nanoalloys for all nanoparticle compositions. Strong improvement of the oxidation resistance resulted from the increase of the atomic gold fraction in the nanoparticles. At gold fractions above 0.4, most of the nanoparticle oxidation was quenched, inhibiting the release of toxic silver ions in solution. The oxidation of the produced nanoparticles was mainly attributed to the generation of free radicals (O•, H•, •OH) and of molecular reactive oxygen species (O2, H2, H2O2) formed by the decomposition of the water molecules through femtosecond laser-induced optical breakdown. For some biological applications, like surface-enhanced Raman spectroscopy (SERS), it is anticipated that AuAg nanoalloys would be the best compromise in terms of chemical stability and plasmonic response, as they possess much better resistance to oxidation in comparison to pure silver and a much stronger and narrower plasmon peak in comparison to pure gold. Introduction Nanoparticles (NPs) of noble metals belong to the most extensively studied colloidal system in the field of nanoscience and nanotechnology. Because of their surface plasmon resonance, such particles show extremely high scattering and absorption cross section, much larger than any organic counterpart.1,2 Furthermore, the coupling between the induced field from the oscillating electrons and the incident field gives rise to significant local field amplification near the NPs surface and to drastic enhancement of the Raman scattering as it scales with |E|4.3 Surface-enhanced Raman scattering (SERS) not only is of interest as a method for ultrasensitive detection and characterization of biomolecules4 but also finds applications in the study of cellular processes,5 bioimaging,6 and in the development of sensitive optical probes.7 In most in vivo applications, Au NPs are preferred because of their easy surface functionalization or bioconjugation and their great chemical stability and biocompatibility.8 However, Ag nanostructures normally show much better plasmonic features in comparison to Au nanostructures of similar size and shape, i.e., that they possess stronger molar extinction coefficient and much narrower plasmon line width.9,10 The latter is of significant importance as a narrow line width (or, equivalently, a long plasmon lifetime) is beneficial for all effects relying on large near field enhancement factors.11 Despite these significant advantages, the introduction of Ag NPs for sensing and biomedical applications has been mainly hampered because of known toxicity and protein denaturation issues, both being related to the release of Ag ions and to related oxidative stresses.12-15 Hence, the formation of nanoalloys could potentially be the best compromise between the plasmonic efficiency and in vivo applicability. * To whom correspondence [email protected]
AuAg nanoalloys and core-shell synthesis have already been reported by chemical reduction techniques16,17 and by nanosecond laser-induced alloying of a mixture of pure Au and Ag NPs.18,19 The effect of the composition on the plasmon peak16-19 and on the SERS efficiencies20,21 has also been widely discussed in the literature. However, none of these works studied the NPs chemical stability and resistance to oxidation as a function of the composition, which is of significant importance for biorelated applications. Here we report the formation of AuAg nanoalloys by a femtosecond (fs) laser-based ablation and fragmentation approach and study their resistance to photoinduced oxidation and Ag ions release. This technique allows the formation of nanospheres of chosen composition having the same size and shape in a very simple chemical environment, i.e., water with a surface stabilizing agent. Hence, variations in the environment and in size and shape could be ruled out, greatly simplifying the analysis of the optical and chemical properties. Furthermore, the reduction of the pulse time width allows a selective tuning of the laser energy deposition in the solvent through nonlinear interactions, which enables a better control of the optical breakdown and related reactive oxygen species (ROS) production in comparison to longer laser pulses. Such ROS are of critical importance in the laser alloying process and strongly affect the final nanoparticles composition though oxidative mechanisms. Experimental Methods Instrumentation. The production rate and NPs concentration were determined from the target mass difference before and after the laser ablation process by using an analytical balance with a precision of 0.01 mg. Static UV-vis spectroscopy was performed using an Agilent 8452 UV-vis diode array spectrometer. Dynamic UV-vis spectra during the laser alloying process were acquired by an Ocean Optics USB4000 UV-vis fiber-optic spectrometer. The minimal integration time was 35 ms, corre-
10.1021/jp102461u 2010 American Chemical Society Published on Web 05/20/2010
J. Phys. Chem. C, Vol. 114, No. 23, 2010
sponding to 35 laser pulses. The size of the NPs was determined by a Jeol JEM-2100F microscope operating at 200 kV. Samples for TEM studies were prepared by drying drops of the aqueous colloidal solution on a carbon-coated copper grid at ambient conditions. The mean size was deduced from the measurement of 500-1000 NPs using the software ImagePro Plus. NPs compositions and internal structure were characterized by energy dispersive X-ray spectroscopy (Jeol JEM-2100F) and by X-ray diffraction (Phillips X’PERT). In some experiments, dialysis of the produced nanoparticles was used to eliminate small generated ROS directly after the laser alloying process. It was carried out on a 50 kDa dialysis membrane (Spectrum Laboratories, Inc.) immersed in a 4 L container filled with stirred deionized water. The time of the dialysis was 24 h, and the water was changed every 8 h. Laser Synthesis of Au and Ag NPs. The synthesis of pure Au and Ag NPs was carried by fs laser ablation in an aqueous solution and has been described in details in our previous papers.22-24 The specific laser ablating conditions and instrumentation are summarized here. In brief, the laser system used in this study consisted of a Ti:sapphire laser (Hurricane, Spectra Physics) with a pulse width of 110 fs (fwhm) centered at 800 nm operating at a repetition rate of 1 kHz. The beam profile and z-propagation were measured by a CCD camera (Ophir, Scor-20som), and the laser energy was controlled by using a diffractive variable attenuator (Del Mar Photonics, DVA-800). Motion of the target with respect to the laser beam was provided by a 3-axes motorized stage and allowed a fine-tuning of the laser fluence as well as the surface scanning during the laser ablation process. The output beam was first expanded to 21 mm using a 3X beam expander and then focused by a custom-made microscope objective with a numerical aperture (NA) of 0.12 (WD ) 75 mm) on the surface of a polished metallic target (Au, Ag) placed at the bottom of a glass vial filled with 20 mL of a 1 g/L aqueous dextran (MW ) 500 kDa) solution. The laser fluence was set to 0.3 J/cm2 (E ) 500 µJ, 2ω0 ) 460 µm) by defocusing the laser beam by 2.0 mm with respect to the laser focus on the target surface. To improve the ablation rate and to limit the interaction between the ablated species and subsequent laser pulses, the solution was stirred during the laser ablation process and the height of the liquid layer was limited to 5 mm by using a large surface-to-volume ratio. Under such conditions, the laser ablation resulted in the formation of Au and Ag NPs with a mean size of 3.3 ( 1.5 and 4.4 ( 2.7 nm at a production rate of 0.12 ( 0.01 and 0.039 ( 0.004 mg/min, respectively. Laser-Induced Alloying. In a secondary step, small aliquots of pure Au and Ag colloids were mixed together in another glass vial and then further irradiated by the fs laser pulses. The final composition of the NPs was tuned by adjusting the Au to Ag molar concentration ratio between 0 and 1. Two laser configurations were tested and are schematically represented in Figure 1. In the strong optical breakdown (SOB) configuration, the laser beam was focused using a large NA microscope objective (NA ) 0.12, WD ) 75 mm) through the open exit of a glass vial containing 2 mL of the mixed colloidal solution, which corresponded to a water thickness of 13.5 mm. The laser focus was set at 6.8 mm below the water surface, providing a theoretical beam waist of 2.24 ( 0.02 µm (ω0 @ 1/e2) according to the measured beam propagation. This configuration resulted in the production of a strong optical breakdown in the liquid noticeable by significant bubbles formation and a strong laser scattering before the actual laser focus. In the low optical breakdown (LOB) configuration, the laser beam was focused
Besner and Meunier
Figure 1. Sketch of the experimental setup used in the strong optical breakdown (SOB) configuration and in the low optical breakdown (LOB) configuration. The position of the focal point, the minimal beam waist, and the beam shape in the x-y plane are given as reference.
Figure 2. Maximum extinction coefficient of the Ag colloidal solutions after 20 min of fs laser irradiation in the SOB configuration. Initial maximum extinction is denoted by the horizontal dashed line.
by a plano-convex lens (NA ) 0.034, f ) 100 mm) through the side of a cylindrical glass vial (φouter ) 14.7 mm, φinner ) 13.3 mm) filled with 3 mL of the mixed colloidal solution. As previously noted,25,26 the use of a small NA favored the generation of a supercontinuum from the optical breakdown. Furthermore, the cylindrical vial acted as a secondary lens, which produces a beam of ellipsoidal shape with distinct X and Y focusing position. By using the ABCD formalism in paraxial approximation, the focusing position inside the water layer (zi) and beam waist (ω0i) could be approximated to (zx ) 7.34 mm, ω0xx ) 5.79 µm, ω0xy ) 74.6 µm) and to (zy ) 10.4 mm, ω0yx ) 101 µm, ω0yy ) 7.94 µm) for the X and Y propagation, respectively. Thus, this LOB configuration provided an enlarged focus region with an intensity 90 times lower compared to the SOB configuration for identical pulse energy, significantly reducing the plasma formation through optical breakdown without sacrificing the fragmentation efficiency. Results and Discussion Laser-Induced Ag Ionization. The resistance of pure Ag NPs to fs laser-induced ionization was first studied using the SOB configuration. Figure 2 shows the maximum extinction coefficient of the Ag plasmon peak after 20 min of fs laser irradiation. Two distinct behaviors could be noticed with the increase of the laser intensity. For laser intensity below 6 × 1014 W/cm2, irradiation of the colloids resulted in a significant increase of the extinction coefficient near 400 nm. This increase was accompanied by the formation of a much narrower and symmetrical Ag plasmon peak. Such variations could be ascribed to the fragmentation of large NPs and aggregates present in the
Femtosecond Laser Synthesis of AuAg Nanoalloys
J. Phys. Chem. C, Vol. 114, No. 23, 2010 10405
Figure 3. Effect of dialysis on solution stability. Extinction spectra of the pure Ag colloidal solution before (solid line) and after 20 min of laser irradiation at a laser intensity of 1.7 × 1014 W/cm2 (dashed line) are reported. The extinction spectra after 24 h with (dot) and without dialysis (dotted line) are also given.
initial solution, resulting in the production of a much narrower NP population. Above this threshold, the plasmon peak gradually disappeared with the increase of the laser intensity and led to the formation of a transparent solution for laser intensities above 3.7 × 1015 W/cm2. No Ag deposition could be noticed on the wall of the glass vial during the laser process, and no sedimentation was seen even for prolonged storing time at room temperature. Furthermore, nanoparticles could not be found in TEM, although the presence of Ag could be noticed on the TEM grid by EDS measurements. Hence, we reasoned that under such strong irradiating conditions the Ag NPs were oxidized and decomposed into solvated Ag ions, presumably in the form of silver hydroxide (AgOH), silver oxide (AgO2), and silver peroxides (Ag2O · Ag2O3). The complete restoration of the plasmon peak upon the addition of a strong reducing agent, such as NaBH4, also confirmed the generation of such compounds in solution. According to our data, the reaction rate of the laserinduced oxidation was very high, as the complete loss of the plasmon peak took only few minutes at the highest intensity used in this study. A much slower oxidation process could also be observed after the laser irradiation in the fragmentation regime or LOB configuration. As shown in Figure 3, most of the fragmented species were transformed into ions 24 h after the fs laser processing at 1.7 × 1014 W/cm2. However, this secondary oxidation could be completely quenched if the colloids were dialyzed over the same period. Such result indicated that the postlaser ionization of the Ag NPs was probably due to the formation of small oxidative species during the laser fragmentation process, as the molecular weight cutoff of the membrane (50 kDa) did not allow the separation of the dextran from the Ag NPs. Furthermore, a similar decrease of the plasmon peak intensity could also be observed after the fragmentation of pure Ag NPs in deionized water, discarding the possible ripening or ionization effect of the stabilizing agent.27 Direct laser-induced oxidation and radical-induced oxidation can greatly influence the composition of the Au and Ag alloys produced by fs laser irradiation, since they limit the available quantity of Ag atoms in solution. Furthermore, the composition of the alloy must play a critical role on the oxidation behavior of the particles, as pure Au NPs were not scavenged under similar irradiating conditions. The alloying process in the LOB regime (low intensity, low NA) and in the SOB regime (high intensity, high NA) as well as the resistance of the resulting alloys to oxidation are reported in the next two sections. Alloying Process in the Fragmentation Regime. The alloying process was first tested using the LOB configuration
Figure 4. (a) Extinction spectra of AuAg nanoalloys with varying GMF in solution by using the LOB configuration at 1.7 × 1014 W/cm2. (b) Variation of the plasmon peak position and extinction cross section of the NPs with the change of the GMF in solution for four different essays. Extinction cross section is calculated by assuming a mean size of 5 nm.
at a laser energy of 250 µJ/pulse, which provided a theoretical maximum local intensity of 1.7 × 1014 W/cm2. Figure 4a shows the characteristic extinction spectra of the alloys after 20 min of laser irradiation, and Figure 4b summarizes the plasmon peak position and the extinction cross section obtained for a series of four different essays. As shown in those figures, the plasmon peak position linearly shifted from 398 to 520 nm with the increase of the gold molar fraction (GMF) in solution at a rate of 1.32 ( 0.03 nm/%. Significant increase of the plasmon bandwidth could also be observed with the increase of the GMF. Inversely, the extinction cross section of the NPs by assuming a mean size of 5 nm (see Nanoalloys Characterization) was found to decrease significantly with the increase of the GMF. Furthermore, the absence of the characteristic peaks of the pure Ag and Au NPs in the spectra of the AuxAg(1-x) NPs suggested that the produced structure is rather homogeneous and did not consist of segregated metal forming a core-shell structure.28 Such characteristics are consistent with previous nanoalloys formation by chemical reduction16 and by nanosecond (ns) laser fragmentation.18 Moreover, the general trends in the plasmon modifications with the increase of the GMF, i.e., the linear plasmon peak shift, the increase of bandwidth, and the decrease of the extinction cross section, are well described by taking into account a linear variation of the interband transition energy threshold with the atomic gold fraction (AGF) in the NPs.28 Such results suggested that the AGFs in the NPs were the same as the GMFs in the solution for the nanoalloys produced in the LOB configuration. Note also that the composition-weighted average of the dielectric function assumption often reported in the literature16,19,29 was not able to describe the general features of the plasmon variations with the composition obtained in this study. This assumption led to a much broader and asymmetric plasmonic band, especially for an AGF between 0.6 and 0.9, which was not consistent with our experimental results. Great
J. Phys. Chem. C, Vol. 114, No. 23, 2010
Besner and Meunier
Figure 5. Long-term stability of nanoalloys with varying AGF deduced from the variations of the maximum extinction coefficient at the plasmon peak position. The nanoalloys were produced by using the LOB configuration at 1.7 × 1014 W/cm2.
care must also be taken in the choice of the dielectric function of the pure Au and Ag NPs. For Au, the constants from Johnson and Christy30 provided the best agreement for NPs with size between 20 and 100 nm. For Ag NPs the dielectric constant from Palik31 provided the best agreement, although they still underestimate the contribution of the interband transition to the dielectric function of the small NPs produced in this study. Hence, size dependence of the dielectric function must be taken into account, as initially reported by Kreibig.9 Details of the Mie model will be given elsewhere. A significant difference in the postlaser oxidation of NPs could be noticed for the different nanoalloys. As shown in Figure 5, most of the fragmented Ag NPs were oxidized 4 h after the laser process. After 24 h, only 14% of the Ag NPs remained in the solution. In comparison, the postlaser oxidation rates observed for the nanoalloys significantly decreased with the AGF increase. After the same period, 60% of the Au0.2Ag0.8 and 87% of the Au0.4Ag0.6 nanoalloys survived to the oxidation. For AGF > 0.4, the nanoalloys were completely resistant and did not show any decrease of their population through radicalinduced oxidation. Hence, the introduction of a small amount of Au into the Ag NPs could significantly enhance the biocompatibility of Ag NPs, as their toxicities are mainly related to the release of Ag ions in the physiological environment. Alloying Process in the Ionization Regime. To investigate the resistance of the produced nanoalloys to the direct laserinduced oxidation, the alloying process was also carried in the ionization regime by using the SOB configuration at an intensity of 1.5 × 1016 W/cm2. Figure 6 shows the plasmon characteristics of the alloys obtained by this process. Two distinct behaviors could be observed with the decrease of the GMF in solution. For a GMF between 1 and 0.45, the plasmon peak position shift linearly with a rate of 1.13 ( 0.04 nm/%, which was consistent with the results obtained in the fragmentation regime. However, the linear shift of the plasmon peak below this GMF decreased to 0.41 ( 0.08 nm/%, indicating that the nanoalloys produced in this region were gold-enriched in comparison to the initial amount of gold in solution. The dip in the extinction coefficient of the solution also supports this idea, as the number of remaining NPs is expected to fall if the amount of Au in solution is decreasing faster than the atomic fraction of Au inside the NPs. Such results also indicated that an increased fraction of Ag atoms were loss into ions through laser-induced oxidation with the decrease of the GMF. TEM and energy dispersive X-ray spectroscopy (EDS) data reported in Table 1 confirmed those conclusions. For all nanoalloys, the compositions determined by EDS and the ones obtained from the Mie theory by assuming
Figure 6. (a) Extinction spectra of AuAg nanoalloys with varying GMF in solution by using the SOB laser configuration at 1.5 × 1016 W/cm2. (b) Variation of the plasmon peak position and normalized extinction coefficient with the change of the GMF in solution for five different essays. Error bars show the standard deviation of the measured extinction coefficients from the five different essays.
a linear variation of the plasmon peak with the composition were consistent. The TEM and EDS data also confirmed that the higher wavelength in plasmon peak positions for GMF between 0.1 and 0.4 are effectively due to an increase of the AGF in the NPs and not to discrepancy in size or agglomeration state. It was also very interesting to note that the NPs which survived the direct laser-induced oxidation had a minimal AGF of 0.41, just like in the radical-induced oxidation. Hence, the Au0.4Ag0.6 could be the best compromise in term of chemical stability, biocompatibility, and plasmonic response, as is it much more resistant to oxidation in comparison to pure Ag and possess a much stronger and narrower plasmon peak in comparison to pure Au. Furthermore, the dynamic UV-vis spectroscopy revealed that the formation of AuAg nanoalloys was most likely formed by the diffusion of Ag atoms into pure Au NPs. Indeed, as shown in the Figure 7, the plasmon peak of Au was continuously blueshifting during the laser irradiation process, while the plasmon peak of Ag decreased in intensity but barely shifted. The higher mobility of small Ag atoms in comparison to Au atoms may explain the Ag into Au interdiffusion and the invariance in the Ag plasmon peak position during the laser irradiation process. Such results were consistent with nanosecond laser alloying process made by Compagnini et al.,19 although no evidence of core-shell particles could be found in our case. Nanoalloys Characterization. Characterization by TEM, EDS, and XRD was carried for the nanoalloys produced in LOB and SOB configurations. Figure 8 shows a typical TEM image of the generated nanoalloys with the corresponding size histogram. In fact, the size of all nanoalloys generated in this study was roughly the same for all compositions and laser
Femtosecond Laser Synthesis of AuAg Nanoalloys
J. Phys. Chem. C, Vol. 114, No. 23, 2010 10407
TABLE 1: Mean Size, Plasmon Peak Position, and AGF of the Nanoalloys Estimated by the Mass of Au and Ag Added to Solution, by EDS, and by Assuming a Linear Change of the Plasmon Peak Position with the Composition (MIE)a NPs composition
mean size (nm)
plasmon peak (nm)
0 0.2 0.3 0.4 0.5 0.6 0.8 0.9 1
4.4 ( 2.7 5.2 ( 2.1 6.2 ( 2.0 5.7 ( 1.7
402 ( 2 448 ( 2 454 ( 2 458 ( 2 464 ( 2 472 ( 2 506 ( 2 505 ( 2 522 ( 2
0 0.21 ( 0.01 0.30 ( 0.02 0.40 ( 0.02 0.50 ( 0.03 0.60 ( 0.04 0.81 ( 0.05 0.89 ( 0.05 1
7.2 ( 2.5 5.6 ( 2.0 3.3 ( 1.5
0.41 ( 0.02 0.42 ( 0.04
0.400 ( 0.007 0.450 ( 0.008 0.483 ( 0.008 0.533 ( 0.009 0.60 ( 0.01 0.88 ( 0.02 0.87 ( 0.02
0.55 ( 0.03 0.59 ( 0.13 0.76 ( 0.06 0.84 ( 0.02
The nanoalloys were synthesized by using the SOB configuration at 1.5 × 1016 W/cm2.
Figure 7. Snapshots of the dynamic UV-vis spectroscopy showing the changes in the extinction spectra of a 0.5 GMF in solution upon fs laser irradiation by using the SOB configuration at 1.5 × 1016 W/cm2.
Figure 8. Typical TEM image and size histogram of AuAg nanoalloys produced after 20 min of fs laser irradiation in the SOB configuration. The AGF of the nanoalloy is 0.4.
intensities. This phenomenon was attributed to the presence of an excess of dextran in solution, which inhibited the growth of the NPs after their fragmentation. In such excess conditions, the final size depended mainly on the affinity between the dextran and the NPs. For Ag and Au, this affinity is the same and restricted the mean size of the NPs between 5 and 7 nm in both laser configurations. The weak dextran-nanoparticle interaction also enables a very efficient ligand exchange with other polymers such as thiolated poly(ethylene glycol) (PEGSH), providing an easy pathway for surface bioconjugation. The presence of fringes in HRTEM also indicated that the produced NPs were crystalline, although some twinned plane and defects could be observed. Further characterization of the produced colloids by XRD (Figure 9) revealed that the nanoalloys possessed a fcc structure, like the pure Au and Ag NPs. As shown in Figure 10, line-EDS scans also confirmed the formation of alloys with an homogeneous spatial atomic
Figure 9. XRD spectra of pure Ag or Au NPs (bottom line) and of the AuAg nanoalloys (top line). The peaks have been assigned to the (111), (200), (220), and (311) crystal planes of the fcc crystal structure.
Figure 10. Spatial AGF measured by line-scan EDS, accompanied by HRTEM image showing the individual lattice planes, as well as the defect structures of the nanoalloys (GMF ) 0.8).
distribution, as previously suggested by the extinction spectra of the colloidal solutions. Again, such results were very general and were applicable to all nanoalloys produced, irrespective of the atomic composition. Hence, the change in the oxidation resistance of the Au-enriched Ag NPs was probably due to a change in their intrinsic chemical properties rather than to a change in their morphological or crystalline structure. Mechanisms of Ag Ionization. For fs laser pulses, significant laser energy deposition in the water medium occurs when the laser intensity is greater than the optical breakdown threshold defined as 1.11 × 1013 W/cm2.32 Above this threshold, the ultrafast laser pulse will ionize and dissociate the water molecules mostly through multiphoton ionization.33 Nanoplasma generated in the close proximity of the plasmonics nanostructures could also contribute to the dissociation of the water molecules at lower laser intensity because of the near-field amplification effects.34 This would lead to the generation of O•, H•, and •OH radicals following the recombination of the
J. Phys. Chem. C, Vol. 114, No. 23, 2010
produced ions with free electrons.35 The oxidation potentials of O• (2.42 V) and •OH (2.80 V) radicals are much larger than the oxidation potential of Ag0 (0.8 V) and would therefore be able to oxidize the Ag atom into silver oxide or silver hydroxides, respectively. Similar electron transfer reaction from Ag to the halogens was reported in the literature.36 However, the lifetime of such radicals is very short, and their action should be seen only during a short period following the fs laser pulse and plasma formation. For instance, the lifetime of hydroxyl radical in water is about 2 ns.37 For the oxygen radical, the lifetime is of the order of a few microseconds or less.38 Those radicals would then form O2, H2, and H2O2 very rapidly upon collisions. The formation of such compounds by intense fs laser pulses was already confirmed by gas chromatography and by mass spectroscopy.35,39 In our case, we verified the presence of H2O2 by using a photometric analysis of the intense yellow color appearing in the solution after the addition of titanium sulfate. The resulting peroxotitanyl complex showed a broad peak centered at 410 nm, which was directly proportional to the quantity of peroxide in solution. The peroxide was also quite long-lived, as the formation of peroxotitanyl complexes was attested even if the addition of titanium sulfate was made weeks after the laser process with or without the presence of NPs in the LOB or SOB configuration. The catalytic reaction between the peroxide and the Ag NPs would then be responsible for the decomposition of the Ag NPs seen after the laser irradiation.40 As the production of ROS is the direct result of the water decomposition from the optical breakdown, their number should increase with the laser intensity, which would lead consequently to an increase of the oxidation rate of the Ag NPs in solution. Increase in the laser intensity would also increase the volume of the laser-induced plasma and therefore the volume of interaction between the free radicals and the NPs in solution. The radicals being much more reactive in comparison to the peroxide, they could possibly account for the much stronger oxidation rate seen at the highest intensities used in this study. However, it is noteworthy to mention that we did not observe such oxidation in the case of nanosecond laser irradiation (τ ) 5 ns, f ) 10 Hz, λ ) 532 nm) with or without laser focusing, irrespectively of the pulse energy (results not shown). As previously demonstrated, ns laser can produce much stronger optical breakdown near the focal point.32 Electron-ions recombination in the plasma would therefore lead to the formation of free radicals just like in the case of fs laser irradiation. On the other hand, the production of H2O2 is normally inhibited in ns laser irradiation due to its dissociation by successive shock waves produced by the plasma35 Hence, these results corroborate the fact that peroxide should be the main oxidative agent observed in our experiments. According to such oxidation mechanisms, the strong increase in the oxidation resistance observed with the increase of the AGF inside the NPs could probably result from significant modifications of the electrochemical properties of the NPs. In fact, no change could be noticed in the general morphological/ crystallographic features of the nanoalloys with the composition. Furthermore, Ag and Au significantly differ in their electronic properties. In this respect, colloidal Ag NPs are known to act as an electron storage (donor) medium.41 Hence, they would easily dissociate through an anodic reaction to release an electron and an Ag+ ions.36 In contrast, Au is known to possess some electron acceptor properties.42 The addition of Au atoms inside the Ag NPs would then contribute to the formation of internal electron traps, inhibiting the dissolution of Ag NPs and the release of Ag+ ions. The dissolution of silver atoms into silver
Besner and Meunier ions being a one electron process, our results also suggest that gold atoms could accommodate slightly more than one electron, as the oxidation was quenched for an AGF between 0.4 and 0.5. Furthermore, although we reason that the ROS formed by the laser process should be the main cause of the Ag oxidation, direct laser-induced photo-oxidation of the Ag NPs cannot be completely ruled out for large laser intensities. Actually, thermionic emission leading to the Coulomb explosion of Au NPs and to ions release has been demonstrated for nanosecond laser pulses.43 As silver possesses a smaller work function in comparison to gold, it is anticipated that Ag should be much more sensitive to photo-oxidation. Furthermore, it was shown that the self-influence of the fs laser beam via the generation of the second harmonics by metallic nanoclusters, and its good matching to Ag plasmon resonance would enhance the laser energy deposition into such NPs in comparison to Au.44 In our case, dynamic UV-vis spectroscopy revealed a much faster change of the extinction spectra of the Ag colloidal solution in comparison to the Au colloidal solution for the same irradiating parameters, indicating a better coupling of the laser energy to Ag NPs. Hence, the lower energy transfer efficiency and the higher ionization threshold of Au NPs could also explain why Au NPs were much more stable under described irradiating conditions. Conclusion We developed a fs laser-based approach for the production of homogeneous AuAg nanoalloys. This unique technique allowed the formation of nanoalloys of various compositions with a constant size in a very simple chemical environment, greatly simplifying the physicochemical analysis of the NPs. Strong increase in the oxidation resistance was observed with the increase of the Au atomic fraction inside the NPs, which was attributed to a significant change of the electron transfer properties of the nanoalloys with the composition. At gold fractions above 0.4, most of the AuAg NPs oxidation was quenched, which inhibited the release of potentially toxic Ag ions in solution. Hence, silver NPs enriched with a low gold molar fraction could significantly surpass pure Au or Ag NPs, as they exhibit much more stability in comparison to silver and higher plasmonic response in comparison to gold. Nanoparticles with higher gold content could also be beneficial for SERS applications as the overall amplification factors depend not only on the intrinsic nanoparticles properties but also on the overlap between the plasmon peak position, the excitation source, and the absorption spectra of the probed molecule. Furthermore, the fs laser-induced optical breakdown was shown to produce free radicals, as well as ROS, which could be of great interest for sterilization in medical and biological applications, although they were detrimental for the production of stable silver-rich NPs. Their production nevertheless mimicked the presence of ROS in biological medium and gave an insight into biocompatibility of such nanoalloys.15 Cytotoxicity studies of the AuAg nanoalloys as a function of the composition are currently underway and will be published elsewhere. Acknowledgment. The authors acknowledge the financial contribution from the Natural Science and Engineering Research Council of Canada (NSERC), the Canadian Institute for Photonics Innovations (CIPI), and the NSERC Strategic Network for Bioplasmonic Systems (BiopSys). We also thank J.-P. Sylvestre and A. V. Kabashin for fruitful discussions and Y. Drolet, S. Poulin, and J.-P. Masse for technical help.
Femtosecond Laser Synthesis of AuAg Nanoalloys References and Notes (1) Yguerabide, J.; Yguerabide, E. E. Light-Scattering Submicroscopic Particles as Highly Fluorescent Analogs and Their Use as Tracer Labels in Clinical and Biological Applications - I. Theory. Anal. Biochem. 1998, 262, 137–156. (2) Boisselier, E.; Astruc, D. Gold Nanoparticles in Nanomedicine: Preparations, Imaging, Diagnostics, Therapies and Toxicity. Chem. Soc. ReV. 2009, 38, 1759–1782. (3) Weitz, D. A.; Garoff, S.; Gersten, J. I.; Nitzan, A. The Enhancement of Raman Scattering, Resonance Raman Scattering, and Fluorescence from Molecules Adsorbed on a Rough Silver Surface. J. Chem. Phys. 1983, 78, 5324–5338. (4) Kneipp, K.; Kneipp, H.; Itzkan, I.; Dasari, R. R.; Feld, M. S. Ultrasensitive Chemical Analysis by Raman Spectroscopy. Chem. ReV. 1999, 99, 2957–2975. (5) Zhang, X. L.; Yin, H. B.; Cooper, J. M.; Haswell, S. J. Characterization of Cellular Chemical Dynamics Using Combined Microfluidic and Raman Techniques. Anal. Bioanal. Chem. 2008, 390, 833–840. (6) Eliasson, C.; Loren, A.; Engelbrektsson, J.; Josefson, M.; Abrahamsson, J.; Abrahamsson, K. Surface-Enhanced Raman Scattering Imaging of Single Living Lymphocytes with Multivariate Evaluation. Spectrochim. Acta, Part A 2005, 61, 755–760. (7) Nguyen, C. T.; Nguyen, J. T.; Rutledge, S.; Zhang, J.; Wang, C.; Walker, G. C. Detection of Chronic Lymphocytic Leukemia Cell Surface Markers Using Surface Enhanced Raman Scattering Gold Nanoparticles. Cancer Lett. 2010, 292, 91–97. (8) Sperling, R. A.; Parak, W. J. Surface Modification, Functionalization and Bioconjugation of Colloidal Inorganic Nanoparticles. Philos. Trans. R. Soc. London A 2010, 368, 1333–1383. (9) Kreibig, U.; Vollmer, M. Optical Properties of Metal Clusters; Springer: Berlin, 1995. (10) Plieth, W.; Dietz, H.; Anders, A.; Sandmann, G.; Meixner, A.; Weber, M.; Kneppe, H. Electrochemical Preparation of Silver and Gold Nanoparticles: Characterization by Confocal and Surface Enhanced Raman Microscopy. Surf. Sci. 2005, 597, 119–126. (11) Messinger, B. J.; von Raben, K. U.; Chang, R. K.; Barber, P. W. Local Fields at the Surface of Noble-Metal Microspheres. Phys. ReV. B 1981, 24, 649–657. (12) Lok, C. N.; Ho, C. M.; Chen, R.; He, Q. Y.; Yu, W. Y.; Sun, H.; Tam, P. K. H.; Chiu, J. F.; Che, C. M. Silver Nanoparticles: Partial Oxidation and Antibacterial Activities. J. Biol. Inorg. Chem. 2007, 12, 527–534. (13) Ayala-Nu´n˜ez, N.; Lara Villegas, H.; del Carmen Ixtepan Turrent, L.; Rodrı´guez Padilla, C. Silver Nanoparticles Toxicity and Bactericidal Effect against Methicillin-Resistant Staphylococcus Aureus: Nanoscale Does Matter. NanoBiotechnology 2009, 5, 2–9. (14) Arora, S.; Jain, J.; Rajwade, J. M.; Paknikar, K. M. Cellular Responses Induced by Silver Nanoparticles: In Vitro Studies. Toxicol. Lett. 2008, 179, 93–100. (15) Li, N.; Xia, T.; Nel, A. E. The Role of Oxidative Stress in Ambient Particulate Matter-Induced Lung Diseases and Its Implications in the Toxicity of Engineered Nanoparticles. Free Radical Biol. Med. 2008, 44, 1689–1699. (16) Link, S.; Wang, Z. L.; El-Sayed, M. A. Alloy Formation of GoldSilver Nanoparticles and the Dependence of the Plasmon Absorption on Their Composition. J. Phys. Chem. B 1999, 103, 3529–3533. (17) Chen, D. H.; Chen, C. J. Formation and Characterization of AuAg Bimetallic Nanoparticles in Water-in-Oil Microemulsions. J. Mater. Chem. 2002, 12, 1557–1562. (18) Zhang, J.; Worley, J.; Denommee, S.; Kingston, C.; Jakubek, Z. J.; Deslandes, Y.; Post, M.; Simard, B.; Braidy, N.; Botton, G. A. Synthesis of Metal Alloy Nanoparticles in Solution by Laser Irradiation of a Metal Powder Suspension. J. Phys. Chem. B 2003, 107, 6920–6923. (19) Compagnini, G.; Messina, E.; Puglisi, O.; Cataliotti, R. S.; Nicolosi, V. Spectroscopic Evidence of a Core-Shell Structure in the Earlier Formation Stages of Au-Ag Nanoparticles by Pulsed Laser Ablation in Water. Chem. Phys. Lett. 2008, 457, 386–390. (20) Rycenga, M.; Hou, K. K.; Cobley, C. M.; Schwartz, A. G.; Camargo, P. H. C.; Xia, Y. N. Probing the Surface-Enhanced Raman Scattering Properties of Au-Ag Nanocages at Two Different Excitation Wavelengths. Phys. Chem. Chem. Phys. 2009, 11, 5903–5908. (21) Yang, Y.; Shi, J. L.; Kawamura, G.; Nogami, M. Preparation of Au-Ag, Ag-Au Core-Shell Bimetallic Nanoparticles for Surface-Enhanced Raman Scattering. Scr. Mater. 2008, 58, 862–865.
J. Phys. Chem. C, Vol. 114, No. 23, 2010 10409 (22) Kabashin, A. V.; Meunier, M. Synthesis of Colloidal Nanoparticles During Femtosecond Laser Ablation of Gold in Water. J. Appl. Phys. 2003, 94, 7941–4943. (23) Sylvestre, J. P.; Kabashin, A. V.; Sacher, E.; Meunier, M. Femtosecond Laser Ablation of Gold in Water: Influence of the LaserProduced Plasma on the Nanoparticle Size Distribution. Appl. Phys. A: Mater. Sci. Process. 2005, 80, 753–758. (24) Kabashin, A. V.; Meunier, M. Femtosecond Laser Ablation in Aqueous Solutions: A Novel Method to Synthesize Non-Toxic Metal Colloids with Controllable Size. J. Phys. Conf. Ser. 2007, 59, 354–359. (25) Besner, S.; Kabashin, A. V.; Meunier, M. Fragmentation of Colloidal Nanoparticles by Femtosecond Laser-Induced Supercontinuum Generation. Appl. Phys. Lett. 2006, 89, 233122(1)233122(3) . (26) Besner, S.; Kabashin, A. V.; Winnik, F. M.; Meunier, M. Synthesis of Size-Tunable Polymer-Protected Gold Nanoparticles by Femtosecond Laser-Based Ablation and Seed Growth. J. Phys. Chem. C 2009, 113, 9526– 9531. (27) Prasad, B. L. V.; Stoeva, S. I.; Sorensen, C. M.; Klabunde, K. J. Digestive-Ripening Agents for Gold Nanoparticles: Alternatives to Thiols. Chem. Mater. 2003, 15, 935–942. (28) Gaudry, M.; Lerme, J.; Cottancin, E.; Pellarin, M.; Vialle, J. L.; Broyer, M.; Prevel, B.; Treilleux, M.; Melinon, P. Optical Properties of (Auxag1-X)(N) Clusters Embedded in Alumina: Evolution with Size and Stoichiometry. Phys. ReV. B 2001, 64, 085407(1)-085407(7). (29) Mulvaney, P. Surface Plasmon Spectroscopy of Nanosized Metal Particles. Langmuir 1996, 12, 788–800. (30) Johnson, P. B.; Christy, R. W. Optical Constants of the Noble Metals. Phys. ReV. B 1972, 6, 4370–4379. (31) Palik, E. D. Handbook of Optical Constants of Solids; Academic Press: Orlando, 1985. (32) Vogel, A.; Noack, J.; Nahen, K.; Theisen, D.; Busch, S.; Parlitz, U.; Hammer, D. X.; Noojin, G. D.; Rockwell, B. A.; Birngruber, R. Energy Balance of Optical Breakdown in Water at Nanosecond to Femtosecond Time Scales. Appl. Phys. B: Lasers Opt. 1999, 68, 271–280. (33) Crowell, R. A.; Bartels, D. M. Multiphoton Ionization of Liquid Water with 3.0-5.0 Ev Photons. J. Phys. Chem. 1996, 100, 17940–17949. (34) Takeda, Y.; Kondow, T.; Mafune, F. Degradation of Protein in Nanoplasma Generated around Gold Nanoparticles in Solution by Laser Irradiation. J. Phys. Chem. B 2006, 110, 2393–2397. (35) Chin, S. L.; Lagace, S. Generation of H2, O2, and H2o2 from Water by the Use of Intense Femtosecond Laser Pulses and the Possibility of Laser Sterilization. Appl. Opt. 1996, 35, 907–911. (36) Tsuji, T.; Okazaki, Y.; Tsuji, M. Photo-Induced Morphological Conversions of Silver Nanoparticles Prepared Using Laser Ablation in Water - Enhanced Morphological Conversions Using Halogen Etching. J. Photochem. Photobiol. A 2008, 194, 247–253. (37) Gupta, S. B.; Bluhm, H. Pulsed Underwater Corona Discharges as a Source of Strong Oxidants: Oh and H2o2. Water Sci. Technol. 2007, 55, 7–12. (38) Yamatake, A.; Fletcher, J.; Yasuoka, K.; Ishii, S. Water Treatment by Fast Oxygen Radical Flow with Dc-Driven Microhollow Cathode Discharge. IEEE Trans. Plasma Sci. 2006, 34, 1375–1381. (39) Nakamura, T.; Mochidzuki, Y.; Sato, S. Fabrication of Gold Nanoparticles in Intense Optical Field by Femtosecond Laser Irradiation of Aqueous Solution. J. Mater. Res. 2008, 23, 968–974. (40) Endo, T.; Yanagida, Y.; Hatsuzawa, T. Quantitative Determination of Hydrogen Peroxide Using Polymer Coated Ag Nanoparticles. Measurement 2008, 41, 1045–1053. (41) Henglein, A. Colloidal Silver Nanoparticles: Photochemical Preparation and Interaction with O-2, Ccl4, and Some Metal Ions. Chem. Mater. 1998, 10, 444–450. (42) Richter, H.; McCarthy, K.; Nevin, K. P.; Johnson, J. P.; Rotello, V. M.; Lovley, D. R. Electricity Generation by Geobacter Sulfurreducens Attached to Gold Electrodes. Langmuir 2008, 24, 4376–4379. (43) Shoji, M.; Miyajima, K.; Mafune, F. Ionization of Gold Nanoparticles in Solution by Pulse Laser Excitation as Studied by Mass Spectrometric Detection of Gold Cluster Ions. J. Phys. Chem. C 2008, 112, 1929– 1932. (44) Shafeev, G. A.; Freysz, E.; Bozon-Verduraz, F. Self-Influence of a Femtosecond Laser Beam Upon Ablation of Ag in Liquids. Appl. Phys. A: Mater. Sci. Process. 2004, A78, 307–309.